Compositions and method for viscosity-increasable dental composites

ABSTRACT

Described is a stable, two-component low viscosity composite that is capable to achieve excellent adaptation to walls/substrates due to its intrinsic flow ability and is also capable of rapid viscosity increasing and being manipulated prior to cure by light upon mixing of such a two-paste composite due to one distinguished reaction promoting partial network formation thus to allow a practitioner further manipulate a firm composite. Upon a completed manipulation by the practitioner, such a mixed material should be readily cured into final solid form by using conventional curing light.

TECHNICAL FIELD

Disclosed herein is a two-component flowable composite that is intrinsically capable of adapting to tooth substrates. In addition, by incorporating a “Chemical Thickener” in two-component flowable compositions, of which would allow two orthogonal chemistries, nucleophile-initiated thiol/ene Michael addition and light-initiated radical polymerization to proceed sequentially. Thus it could to offer the advantage of further manipulation on such thickening paste with adequate working time prior to final curing by light.

BACKGROUND

SureFil SDRflow® set up as a standard for bulk-fill flowable as easy to use and excellent adaption due to its lower viscosity, lower curing stress and high depth of cure. However, it seems highly desirable if it can be further manipulated by the clinicians although the low viscosity make possible to achieve the best adaption, which is critical to minimize the failure of the bulk restoration. Therefore, in order to improve the SureFil SDRflow® while carry its signature feature of self-leveling, a possible phase change from lower viscosity to higher viscosity become a new twist. It is expected that this would be able to effectively balance between adaptation and manipulation.

A flowable composite should be able to undergo a rheological phase change from low viscosity to a firm paste upon a paste/paste mixing. Several approaches were proposed based on either chemistry and/or technology. If a chemistry could allow a selective cure for part of formulated material to building up its texture (viscosity) in given time, it should be possible to develop such a viscosity-increasable flowable that should delivery some feature we would like. For instance, a chemical approach can be based on a sequential curing mechanism, from which distinguished chain growth and network-formation are involved in. Consequently the initial paste offer lower viscosity for achieving good adaptation and then first curing mechanist is triggered for viscosity building-up but would not cause unnecessary cross-linking. Finally cross-linking is kicked in by light irradiation for strengthening the performance.

BRIEF DESCRIPTION OF THE DRAWINGS

FIG. 1 is a schematic of an in situ interpenetrating polymer network process with orthogonal chemistries.

FIG. 2 demonstrates a mechanism for the base-catalyzed thiol-Michael addition reaction.

FIG. 3 demonstrates a thiol/ene reaction to network formation based on PETMP and TCDCDA in the presence of DBU.

FIG. 4 is a visual illustration of the viscosity increasing composite as dual-cure with unlimited working time demonstrating that the viscosity increased as quickly as five minutes.

FIG. 5 shows paste status as different times for an individual paste and a paste/paste mix according to the present disclosure with a metal bearing therein to show the increase in viscosity. The individual paste is on the left of each picture, while the paste/paste mix is shown on the right. As seen from these pictures, the paste/paste mix increases in viscosity at a much faster rate an individual paste alone.

FIG. 6 demonstrates the effect of reactive acrylate resins on the initial viscosity of mixed composites.

FIG. 7 is a schematic of a molecular structure of Ethoxylated-Trimethylolpropane Tri(3-Mercaptopropionate).

FIG. 8 shows the aging effect on viscosity of a conventional TPH® resin system.

FIG. 9 shows the aging effect on viscosity of various mixed resin systems.

FIG. 10 shows the viscosity of TPH® and SDR® resins with various additives.

FIG. 11 is a schematic of molecular structures of thiol inhibitors.

FIG. 12 shows the aging effect on viscosity of THIOCURE PETMP with various resins.

FIG. 13 demonstrates the aging effect on viscosity of various resin mixes with PETMP.

FIG. 14 demonstrates the aging effect on viscosity of THIOCURE PETMP with various resins.

FIG. 15 demonstrates the aging effect on viscosity of TPH Resin, SDR Resin, Isosorbide Resin and EBPADMA as matrix resins in formulations for the catalyst composite paste, in which a hyperbranched polyester acrylate resin (NC2303 from Sartomer) was used as the polyene.

FIG. 16 demonstrates the aging effect on viscosity of a EBPADA/PETMP mix and a UDMA/PETMP mix.

FIG. 17 demonstrates the aging effect on viscosity of various resins with PETMP or ETTMP.

FIG. 18 demonstrates the aging effect on viscosity of various resins with PETMP.

FIG. 19 demonstrates the oscillation profile of SureFil SDRflow®.

FIG. 20 demonstrates the oscillation profile of TPH3®.

FIG. 21 demonstrates the oscillation profile for viscosity increasing flowable formulations.

FIG. 22 demonstrates the oscillation profile for other viscosity increasing flowable formulations.

FIG. 23 demonstrates the oscillation profile for yet other viscosity increasing flowable formulations.

FIG. 24 demonstrates the oscillation profile for yet further viscosity increasing flowable formulations.

FIG. 25 demonstrates the viscosity and storage modulus for various viscosity increasing flowable composites.

ABBREVIATION KEY

-   TEGDMA: tri(ethylene glycol) dimethacrylate -   EDAB: ethyl 4-(dimethylamino) benzoate -   PETMP: Pentaerythritol Tetra(3-mercaptopropionate) -   ETTMP: Ethoxilated-Trimethylolpropan Tri(3-Mercaptopropionate) -   EBPADMA: ethoxylated bisphenol-A dimethacrylate -   TCDCDA: Tricyclo[5.2.1.0²′⁶]decanedimethanol diacrylate -   CQ: camphorquinone -   LTPO: 2,4,6-trimethylbenzoyl-diphenyl-phosphine oxide -   BHT: Butylated hydroxytoluene -   BAFG: barium-alumino fluoroborosilicate glass -   DBU: 1,8-Diazabicyclo[5.4.0]undec-7-ene -   DBN: 1,5-Diazabicyclo[4.3.0]non-5-ene -   TEA: triethylamine -   PYG: Pyrogallol -   TPP: Triphenyl phosphite -   DABCO: 1,4-diazabicyclo[2,2,2]-octane

Test Methods:

NMR Analysis: Nuclear magnetic resonance (NMR) spectra were recorded on a Varian 300 MHz spectrometer. Samples were prepared in CDCl₃ at ca. 15% v/v. Chemical shifts are reported in parts per million (ppm) relative to TMS.

FTIR Analysis: Fourier transform infrared spectra (FTIR/ATR) were recorded on a Thermo Electron Nicolet 6700 Spectrometor.

Photo DSC: Differential Scanning calorimeter (Q2000, TA Instrument) with photocalorimetry accessory (PCA), from which UV/Visible light (250-650 nm) from a 200 W high pressure mercury source is transmitted to the sample chamber via an extended range, dual-quartz light guide with neutral density or band pass filters, was used to evaluate the photolysis and photopolymerization for the neat resin and/or any formulated resin system. Under both air and nitrogen, the test was performed. The light outputs and light spectrum can be tuned by using build-in filter, or additional UV filter or intensity-reducing filter.

Flexural strength and modulus are tested according to ISO 4049, 2×2×25 mm specimens were cured by three overlapped spot curing with Spectrum 800 with 13 mm light guide at 800 mw/cm², 20″ for each spot on one side only. The cured specimens (6-10) were placed in DI water and stored at 37° C. for 24 hrs, then were sanded prior to the test at room temperature.

Compressive strength and modulus are tested according to ISO 9917, which is actually for water-based cements since ISO 4049 does not specify for compressive strength. ϕ4×6 mm glass slave as mold for specimen preparation (6). It was cured by Spectrum 800 at 800 mw/cm² from both top and bottom, at 20″ each. The cured specimens (6-10) were placed in DI water and stored at 37° C. for 24 hrs, and then were sanded prior to the test at room temperature.

Shrinkage Stress was measured by using NIST/ADA's tensometer. Specimen with 2.25 mm in thickness (c-factor as 1.33) is cured for 60 seconds by DENTSPLY/Caulk's QHL light at 550 mw/cm2. The total stress at the 60^(th) minute is taken to rank different materials.

Rheology property was measured by using TA's DHR Rheometor. ϕ40 mm 2° geometry is used for resin viscosity measurement and ϕ20 mm flat geometry was used for composite's evaluation. Oscillation test is set up at 175 Ps shear stress, 1 Hz shear frequency at 35° C.

Ross planetary mixer (120 F/20 in psi), SpeedMix (RT) and Resodyn (RT/20 In psi) are used in prepared filler blend and resin mixture and the flowable composite pastes.

digi syringe system with auto mixing tip was used to pack the individual base paste and catalyst paste, respectively.

DETAILED DESCRIPTION

There are different approaches based on either chemistry and/or technology in creating a viscosity-increasable flowable composite. If chemistry could allow a selective reaction for part of a formulated material to building up its texture (viscosity) in given time, it should be possible to develop such a viscosity-increasable flowable that should delivery some desirable features. For instance, a chemical approach can be based on a sequential curing mechanism, from which distinguished chain growth and network-formation are involved in. Consequently the initial paste offers lower viscosity for achieving good adaptation and then a first curing mechanism is triggered for viscosity building-up but would not cause unnecessary cross-linking. Finally cross-linking is initiated by light irradiation for strengthening the performance.

One example of conventional approach was based on a polyacid/polybase for such viscosity-increasing process, which was indeed able to promote viscosity increasing via non-radical reaction. It was found that the pair of acid/base in structure and composition would impact significantly on the viscosity profile and mechanical property. 10-MDP and Penta appear more effective to react with polyimidazole. Polyacrylic acid showed limited reactivity towards polyimidazole in absence of water. In addition, as expected, a significant increase in water absorption in all cured composites were found, which led to decrease in mechanical strength in wet specimen.

The potential benefits, however, are the improved moisture tolerant as such increased hydrophilicity. In addition, there was also challenge to achieve really good initial adaptation of the resulting as-mixed composite as required from the low viscosity and rapid viscosity increase to allow some kind manipulation plus offer adequate mechanical properties. It should be possible to achieve a balance between viscosity change and paste manipulation but it is also realized that it is remain very challenge for achieving superior mechanical strength as universal composite due to its intrinsic low filler loading without a significant change in filler. In order to achieve a rapid viscosity building-up, new polybase or polyacid resins or reactive filler might be necessary.

Another possible approach to realizing a dual-cure, viscosity-increasing process as described in the present disclosure would be a thiol/ene-based cure for initial chain extension for viscosity building-up while the paste remain as workable/manipulatable, then light irradiation to lead a fully cured material. It was expected that such two distinct chemistries would afford two-stage curing process so as to balance the adequate initial adaptation and subsequent manipulation from a single material. In addition, it was also expected that his approach would address the issues that were noticed in the conventional polyacid/polybase process, such as the increasing water absorption for inferior mechanical properties, relatively slow reaction and an initial higher viscosity. Chris Bowman's team at University of Colorado reported two-stage reactive polymer network forming systems, in which a base-catalyzed thiol-ene addition was set up for initial curing process and photo-initiated light curing to finalize the entire networking process, as shown in FIG. 2. Such chemistry might work for our intended viscosity-increasing flowable composition. However, the thiol-ene reaction is too slow to generate significant viscosity building up. Though a highly reactive super base (1, 8-diazabicyclo [5,4,0]undec-7-ene, DBU) could be used to accelerated the thiol/ene reaction, it was discovered it would also even trigger the methacrylate/thiol reaction for most methacrylate pair we tested, especially for those urethane-based methacrylate resins.

From our comprehensive investigation on such thiol/ene systems, it was further discovered a remarkably stable pare that is composed of dimethacrylate and polytiol, more specifically EBPADMA and PETMP, which would allow to formulate a stable catalyst resin/paste with inclusion of DBU. Furthermore, a viscosity-increasing flowable should be readily resulted from a base paste that is composed of methacrylate resin and polyacrylate resins and photoinitiators for the 2^(nd) step curing; and a catlystat paste that is composed of polytiol and methacrylate matrix and the catalysts of thiol/ene addition, DBU.

As an example, it was illustrated in FIG. 3, a tetrathiol (PETMP) could be used as polythiol and a diacrylate (TCDCDA) or a tetra-acrylate (SR295) was used as polyacrylate, and various bases could be used as catalyst, including triethyl amine (TEA), 1,8-diazabicyclo[5,4,0] undec-7-ene (DBU), and 1,4-diazabicyclo[2,2,2]-octane (DABCO).

As shown in Table 1 when the resin compositions of polythiol resin (PETMP) and polyacrylate resin (TCDCDA or SR295) varied, the speed of viscosity increasing upon mixing the resin blend of PETMP in TPH resin and TCDCDA or SR295 in TPH Resin would change dramatically depending upon the the nature of the base catalyst (DBU, TEA and DABCO). Thus it did indicate that thiol-ene chemistry appears to proceed well and feasible to trigger the stage one network forming process for a viscosity-increasing composite without involving any radical polymerization. It was further found that only 0.3-0.4% of DBU is necessary to have a reasonable networking process for PETMP/TCDCDA system, from which DBU was discovered as the most effective catalyst for such thiol/ene reaction.

TABLE 1 Compositions Effect on Speed of Gelation of Various Thiol-ene Resin Systems Polythiols Polyacrylate Base Catalyst mol mol wt. % Sample ID PETMP TCDCDA SR295 DBU TEA DABCO Gelation Time XJ9-176-1 0.01 0.02 0 0.8 0 0 Instantly solidified XJ9-176-2 0.01 0.02 0 0 0.8 0 3 hours IJ5-170 0.01 0.02 0.1 0.2 4.5 hrs IJ5-171 0.01 0.02 0.2 slower IJ5-172 0.01 0.02 0.2 0.4 1 hr IJ5-173 0.01 0.03 0.3 little faster IJ5-174 0.01 0.04 0.2 0.4 4.5 hrs IJ5-175 0.01 0.04 0.4 Instantly gelation IJ5-176 0.01 0.02 0.2 0.2 3.5 hrs IJ5-177 0.01 0.02 0.2 3-18 hrs IJ5-178 0.01 0.03 0.3 0.2 3-18 hrs IJ5-179 0.01 0.02 0.4 3-18 hrs 175 > 172 > 176 > 170, 174 (177, 178, 179) 170 vs. 176: increasing DBU boost speed of gelation; 172 vs. 176: increasing TEA also boosts speed of gelation; 172 vs. 174: Excessive of TCDCDA decrease speed of gelation 173 vs. 178: Increasing TEA boosts speed of gelation, 171 vs. 175: SR 295 gelation fast than TCDCDA 173 vs. 175: somewhere between 0.3% and 0.4% of DBU change the speed of gelation dramatically.

TABLE 2 Compositions and Viscosities of Formulated Base Resins for Viscosity-increasing Viscosity Resin PETMP ETTMP TPH Resin IsosorbideR SDR UDMA EBPADMA Inhibitors TEGDMA @20° C. Compositions %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt Pa · s IJ5-184 20 80 9-17 IJ5-188 IJ5-192 IJ5-208 IJ6-030 IJ6-055 IJ5-204 20 80 gelled IJ5-206 20 80 gelled IJ6-009 20 80 10  IJ6-008 20 80 2 IJ6-036 IJ6-055 IJ6-073 IJ6-087 IJ6-106 IJ6-113 IJ6-151 IJ6-188 IJ6-020 20 80 PYG/1.00 IJ6-021 20 70 PYG/1.00 10 IJ6-022 20 80 TTBPP/1.00 IJ6-023 20 70 TTBPP/1.00 10 IJ6-024 20 80 TPP/1.00 IJ6-025 20 70 TPP/1.00 10 IJ6-026 20 80 L-Gallate/1.00 IJ6-027 20 70 L-Gallate/1.00 10 IJ6-030 20 80 IJ6-032 20 70 10 IJ6-034 20 70 10 IJ6-036 20 80 2 IJ6-047 20 80 5 IJ7-009 30 70 IJ7-010 25 75 IJ7-047 33 67 IJ7-059 40 60 IJ7-071 IJ7-060 50 50 PYG: Pyrogallol TTBPP: Tris(2,4,-di(tert)-butylpheyl0phosphite TPP: Triphenyl phosphite L-Gallate: Lauryl gallate

TABLE 3 Compositions and Viscosities of Formulated Catalyst Resins for Viscosity-increasing Viscosity Resin TPH Resin CN2303 SR295 TCDCDA CQ BHT LTPO DBU TEA @20° C. Compositions %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt Pa · s IJ5-185 50 50 0.31 0.03 0.80 0.28 2 IJ5-189 50 50 0.21 0.14 2 IJ5-193 70 30 0.31 0.03 0.80 0.56 9 IJ5-194 70 30 0.31 0.03 0.80 0.42 0.28 9 IJ6-051 50 50 0.31 0.03 0.80 0.56 2 IJ6-052 50 50 0.31 0.03 0.80 0.56 5 Viscosity Resin EBPADAM CN2303 IsosorbideR TCDCDA CQ BHT LTPO DBU TEA @20° C. Compositions %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt Pa · s IJ6-053 50 50 0.31 0.03 0.80 0.56 1 IJ6-054 50 50 0.31 0.03 0.80 0.42 0.28 4 IJ6-070 50 50 0.31 0.03 0.80 0.56 6 IJ6-084 50 50 0.31 0.03 0.80 0.84 22 Viscosity Resin EBPADAM SR295 TPH Resin TCDCDA CQ BHT LTPO DBU SDR @20° C. Compositions %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt Pa · s IJ6-071 50 50 0.31 0.03 0.80 0.56 1 IJ6-085 50 50 0.31 0.03 0.80 0.84 2 IJ6-072 50 50 0.31 0.03 0.80 0.56 2 IJ6-069 50 50 0.31 0.03 0.80 0.56 2 IJ6-070 IJ6-083 50 50 0.31 0.03 0.80 0.84 5 IJ6-084 IJ6-086 50 50 0.31 0.03 0.80 0.84 18 IJ6-097 50 50 0.31 0.03 0.80 1.12 2 IJ6-098 50 0.31 0.03 0.80 1.12 50    2 IJ6-099 50 50 0.31 0.03 0.80 1.12 2 IJ6-114 50 50 0.31 0.03 0.80 1.12 2 IJ6-147 50 50 0.31 0.03 0.80 0.86 2 IJ6-148 50 50 0.31 0.03 0.80 0.86 2 IJ6-149 50 50 0.31 0.03 0.80 0.86 EDAB 2 0.40 IJ6-150 50 50 0.31 0.03 0.80 0.86 EDAB 2 0.40 IJ7-007 35 65 0.31 0.80 0.75 EDAB NA 0.40 IJ7-008 35 65 0.31 0.80 0.75 NA IJ7-046 25 75 0.31 0.03 0.80 0.86 EDAB NA 0.40 IJ7-058 35 65 0.31 0.03 0.80 0.86 EDAB NA 0.40 IJ7-070 35 65 0.31 0.03 0.80 0.86 EDAB NA 0.40 Viscosity Resin SR295 TCDCDA IsosorbideR SDR CQ BHT LTPO DBU TEA @20° C. Compositions %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt %, wt/wt Pa · s IJ5-205 30 70 0.31 0.03 0.80 0.42 0.28 35 IJ5-207 30 70 0.163 0.03 0.80 0.42 0.28 52 IJ6-028 50 50 0.31 0.03 0.80 0.07 2 IJ6-100 50 50 0.31 0.03 0.80 1.12 2

Further the flowability of such formulated composition would also vary depending upon the filler and filler content. As showed in Table 2, a variety of flowable compositions with 55-60% wt/wt of fillers was readily formulated by variable DBU contents and different acrylate resins (TDCDDA and SD 295) and different methacrylate resins (TPH resin, SDR resin and Isosorbide Resin). It was also concluded that higher concentration of DBU is more effective than DBU/TEA mixture; and SR295 is more effective than TCDCDA in term of promoting stage one network formation.

Furthermore, as showed in Table 4 and 5, excellent mechanical propertied, flexural strength of 136-152 MPa and flexural modulus of 6750-8200M, could be achieved from such two-stage cure/viscosity-increasing systems. In addition, lower polymerization stress of 2.3-2.8 MP vs. 3.3 MPa were also resulted from such two-stage cure process. Further lower polymerization stress of 2.07 MPa was found upon 90 min delayed light curing process, which indirectly confirmed the stage-one network formation process proceeded. In addition, it was also noted DBU could also act as accelerator for CQ/LTPO photopolymerization as evident by the effective curing under a single-band LED irradiation (IQ2 LED).

It was surprisingly found that both two urethane-based methacrylate resins (isosorbide-based resin and SDR resin) are not chemically compatible with PETMP, as evident by the gelation of IJ5-204 and IJ5-206, respectively. There is no any catalyst presented in these systems and they are all methacrylate resins. Thus it is speculated somehow the impurity in either isosorbide resin or SDR resin can significantly destabilize such thiol-ene system of polylthiol (PETMP) and methacrylates. However, the better stability demonstrated by other urethane-based resin (TPH resin) might suggest that there is no (or less) such “impurity” in TPH resin. Indeed a slow viscosity increasing in TPH resin/PETMP was eventually demonstrated they follow similar trend of instability after it was aged over night at RT though no gel was formed as showed by the viscosity of 17 Pa·s of IJ5-192 vs. 9 Pa·s for those freshly mixed resin blends, IJ5-184, IJ5-188 and IJ5-208. In addition, if freshly mixed isosorbide resin/PETMP or SDR resin/PETMP were immediately formulated into composites (IJ6-001 or IJ6-003 in Table 2), their stability got improved but they still tended to get stiff, which indicated a slower gelation process occurred within the pastes then resin blends.

TABLE 4 Compositions and Properties of Formulated Flowables for Viscosity-increasing Stress @ 60 min Halogen Light Halogen Light Paste Compositions (QHLBlue) Compr. t. (Mpa) Flex. St. (Mpa) Dual Paste Base Paste Catalyst Paste MPa Compr.Mod. (Mpa) Flex. Mod.(Mpa IJ5-186 Resin/IJ5-184 2.83 367 ± 26 145 ± 11 40.05% 2.73 4420 ± 300 7880 ± 600 Filler/XJ8-148 (w/ 1 min delayed) 59.95% 2.61 IJ5-187 Resin/IJ5-185 (w/ 90 min delayed) 41.65% Filler/XJ8-148 58.35% IJ5-190 Resin/IJ5-188 2.81 342 ± 45 152 ± 15 39.95% 2.88 4120 ± 40  8190 ± 470 Filler/XJ8-148 (w/ 1 min delayed) 60.05% 2.07 IJ5-191 Resin/IJ5-189 (w/ 90 min delayed) 44.40% Filler/XJ8-148 55.60% IJ5-195 Resin/IJ5-192 2.31 317 ± 28 136 ± 7  45.01% 3990 ± 370 6750 ± 460 Filler/XJ8-148 54.99% IJ5-196 Resin/IJ5-193 41.65% Filler/XJ8-148 58.35% IJ5-195 Resin/IJ5-192 2.45 333 ± 12 129 ± 4  45.01% 4360 ± 60  6700 ± 400 Filler/XJ8-148 54.99% IJ5-197 Resin/IJ5-194 45.03% Filler/XJ8-148 54.97% IJ6-005 Resin/IJ5-208 2.26 348 ± 18 143 ± 8  45.00% 2.76 (w/ 30 min 3680 ± 320 6780 ± 480 Filler/XJ8-148 delayed) 55.00% IJ6-002 Resin/IJ5-205 45.00% Filler/XJ8-148 55.00% IJ6-005 Resin/IJ6-028 2.59 386 ± 29 140 ± 7  45.00% 2.06 3000 ± 270 7140 ± 130 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-029 Resin/IJ6-030 45.00% Filler/XJ8-148 55.00% IJ6-029 Resin/IJ5-208 2.21 380 ± 12 132 ± 12 45.00% 2.34 3680 ± 320 6550 ± 650 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-037 Resin/IJ6-036 45.00% Filler/XJ8-148 55.00% IJ6-029 Resin/IJ5-208 NA 274 ± 27 126 ± 15 45.00% 2670 ± 260 6350 ± 640 Filler/XJ8-148 55.00% IJ6-048 Resin/IJ6-047 45.00% Filler/XJ8-148 55.00% IJ6-060 Resin/IJ6-055 2.62 274 ± 24 98 ± 7 45.00% 2.64 3370 ± 280 4950 ± 360 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-056 Resin/IJ6-051 45.00% Filler/XJ8-148 55.00% IJ6-060 Resin/IJ6-55 2.56 343 ± 30 106 ± 9  45.00% 2.15 3690 ± 200 4750 ± 280 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-057 Resin/IJ6-052 45.00% Filler/XJ8-148 55.00% IJ6-060 Resin/IJ6-055 2.41 320 ± 35 116 ± 4  45.00% 2.09 3630 ± 380 5280 ± 510 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-058 Resin/IJ6-053 45.00% Filler/XJ8-148 55.00% IJ6-060 Resin/IJ6-73 2.20 330 ± 30 112 ± 4  45.00% 2.15 3590 ± 220 5450 ± 60  Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-059 Resin/IJ6-069 45.00% Filler/XJ8-148 55.00% IJ6-080 Resin/IJ6-73 2.62 261 ± 20 123 ± 12 45.00% 2.64 3950 ± 210 5890 ± 280 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-074 Resin/IJ6-069 45.00% Filler/XJ8-148 55.00% IJ6-092 Resin/IJ6-87 2.21 230 ± 25 124 ± 9  45.00% 2.34 3470 ± 100 6000 ± 300 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-088 Resin/IJ6-083 45.00% Filler/XJ8-148 55.00% IJ6-080 Resin/IJ6-73 2.56 260 ± 30 128 ± 13 45.00% 2.15  4100 ± 1600 6450 ± 180 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-075 Resin/IJ6-070 45.00% Filler/XJ8-148 55.00% IJ6-092 Resin/IJ6-87 2.60 308 ± 35 117 ± 8  45.00% 2.00 3620 ± 330 5070 ± 200 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-089 Resin/IJ6-084 45.00% Filler/XJ8-148 55.00% IJ6-080 Resin/IJ6-73 2.41 299 ± 30 135 ± 8  45.00% 2.09 4180 ± 250 6250 ± 210 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-076 Resin/IJ6-071 45.00% Filler/XJ8-148 55.00% IJ6-092 Resin/IJ6-87 2.86 277 ± 25 119 ± 9  45.00% 2.29 3810 ± 240 4950 ± 480 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-090 Resin/IJ6-085 45.00% Filler/XJ8-148 55.00% IJ6-080 Resin/IJ6-73 2.37 266 ± 20 142 ± 6  45.00% 2.15 3860 ± 100 6330 ± 120 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-077 Resin/IJ6-072 45.00% Filler/XJ8-148 55.00% IJ6-092 Resin/IJ6-87 3.00 280 ± 25 120 ± 4  45.00% 1.58 3770 ± 230 5300 ± 280 Filler/XJ8-148 (w/ 60 min delayed) 55.00% IJ6-091 Resin/IJ6-086 45.00% Filler/XJ8-148 55.00% IJ6-112 Resin/IJ6-106 2.60 206 ± 20 123 ± 9  40.00% 2.46 4000 ± 170 7000 ± 760 Filler/XJ8-148 (w/ 60 min delayed) 60.00% IJ6-108 Resin/IJ6-097 40.00% Filler/XJ8-148 60.00% IJ6-112 Resin/IJ6-106 2.07 230 ± 23 125 ± 14 40.00% 2.39 3200 ± 140 6640 ± 250 Filler/XJ8-148 (w/ 60 min delayed) 60.00% IJ6-109 Resin/IJ6-098 40.00% Filler/XJ8-148 60.00% IJ6-112 Resin/IJ6-106 2.02 228 ± 15 118 ± 12 40.00% 2.06 3550 ± 420 6900 ± 370 Filler/XJ8-148 (w/ 60 min delayed) 60.00% IJ6-110 Resin/IJ6-099 40.00% Filler/XJ8-148 60.00% IJ6-112 Resin/IJ6-106 2.16 230 ± 20 132 ± 3  40.00% 1.72 3550 ± 560 6960 ± 200 Filler/XJ8-148 (w/ 60 min delayed) 60.00% IJ6-111 Resin/IJ6-100 40.00% Filler/XJ8-148 60.00% IJ6-115 Resin/IJ6-113 2.36 270 ± 30 100 ± 10 40.00% 2.37 3750 ± 60  4900 ± 450 Filler/XJ8-148 (w/ 60 min delayed) 60.00% IJ6-116 Resin/IJ6-114 40.00% Filler/XJ8-148 60.00% IJ6-117 Resin/IJ6-113 2.32 195 ± 30 79 ± 7 40.00% 2.36 3960 ± 400 5170 ± 560 Filler/XJ8-148 (w/ 60 min delayed) 60.00% IJ6-118 Resin/IJ6-114 40.00% Filler/XJ8-148 60.00% IJ6-115 Resin/IJ6-113 2.36 270 ± 30 100 ± 10 40.00% 2.37 3750 ± 60  4900 ± 450 Filler/XJ8-148 (w/ 60 min delayed) 60.00% IJ6-116 Resin/IJ6-114 40.00% Filler/XJ8-148 60.00% IJ6-117 Resin/IJ6-113 2.32 195 ± 30 79 ± 7 40.00% 2.36 3960 ± 400 5170 ± 560 Filler/XJ8-148 (w/ 60 min delayed) 60.00% IJ6-118 Resin/IJ6-114 40.00% Filler/XJ8-148 60.00%

TABLE 5 Compositions and Properties of Formulated Flowables for Viscosity-increasing Stress @ 60 min Halogen Light Halogen Light Mixing Dual Paste Composition (QHLBlue) Compr. t.(Mpa) Flex. St.(Mpa) Methods Pastes Base Paste Catalyst Paste MPa Compr. Mod.(Mpa) Flex. Mod.(Mpa SpeedMix IJ6-115 Resin/IJ6-113 2.36 270 ± 30 100 ± 10 40.00% 2.37 3750 ± 60  4900 ± 450 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-116 Resin/IJ6-114 40.00% Filler/XJ8-148 60.00% SpeedMix IJ6-117 Resin/IJ6-113 2.32 195 ± 30 79 ± 7 40.00% 2.36 3960 ± 400 5170 ± 560 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-118 Resin/IJ6-114 40.00% Filler/XJ8-148 60.00% Resodyn IJ6-139 Resin/IJ6-113 2.90 330 ± 20 122 ± 5  40.00% 2.51 3930 ± 340 5110 ± 300 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-140 Resin/IJ6-114 40.00% Filler/XJ8-148 60.00% Resodyn IJ6-141 Resin/IJ6-113 2.78 277 ± 20 104 ± 10 40.00% 2.32 4350 ± 160 5440 ± 420 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-142 Resin/IJ6-114 40.00% Filler/XJ8-148 60.00% RossMixer IJ6-152 Resin/IJ6-147 3.50 295 ± 10 123 ± 12 40.00% 2.94 3800 ± 130 6570 ± 380 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-156 Resin/IJ6-151 40.00% Filler/XJ8-148 60.00% RossMixer IJ6-153 Resin/IJ6-148 3.25 307 ± 10 122 ± 9  40.00% 2.72 3520 ± 180 6910 ± 190 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-156 Resin/IJ6-151 40.00% Filler/XJ8-148 60.00% RossMixer IJ6-154 Resin/IJ6-149 3.65 300 ± 20 130 ± 7  40.00% 2.88 3780 ± 250 6910 ± 400 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-156 Resin/IJ6-151 40.00% Filler/XJ8-148 60.00% RossMixer IJ6-155 Resin/IJ6-150 3.10 300 ± 30 116 ± 6  40.00% 3.47 3800 ± 450 5950 ± 250 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-156 Resin/IJ6-151 40.00% Filler/XJ8-148 60.00% Resodyn IJ6-158 Resin/IJ6-147 2.90 294 ± 30 116 ± 6  40.00% 3.33 3870 ± 270 6080 ± 450 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-162 Resin/IJ6-151 40.00% Filler/XJ8-148 60.00% Resodyn IJ6-159 Resin/IJ6-148 2.78 272 ± 20 126 ± 4  40.00% 3.20 3730 ± 140 5610 ± 400 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-162 Resin/IJ6-151 40.00% Filler/XJ8-148 60.00% Resodyn IJ6-160 Resin/IJ6-149 3.84 286 ± 20 121 ± 7  40.00% 3.06 3560 ± 310 6230 ± 210 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-162 Resin/IJ6-151 40.00% Filler/XJ8-148 60.00% Resodyn IJ6-161 Resin/IJ6-150 3.25 289 ± 15 126 ± 4  40.00% 2.98 3450 ± 300 5970 ± 410 Filler/XJ8-148 (w/30 min 60.00% delayed) IJ6-162 Resin/IJ6-151 40.00% Filler/XJ8-148 60.00% Resodyn IJ7-012 Resin/IJ7-007 3.06 273 ± 20 141 ± 4  35.00% 2.83 4210 ± 210 7570 ± 160 Filler/XJ8-148 (w/30 min 65.00% delayed) IJ7-016 Resin/IJ7-009 35.00% Filler/XJ8-148 65.00% Resodyn IJ7-013 Resin/IJ7-008 2.53 253 ± 20 135 ± 9  35.00% 2.93 3470 ± 230 7530 ± 250 Filler/XJ8-148 (w/30 min 65.00% delayed) IJ7-016 Resin/IJ7-009 35.00% Filler/XJ8-148 65.00% Resodyn IJ7-014 Resin/IJ7-007 3.01 252 ± 20 132 ± 6  35.00% 2.69 3270 ± 200 7470 ± 270 Filler/XJ8-148 (w/30 min 65.00% delayed) IJ7-017 Resin/IJ7-010 35.00% Filler/XJ8-148 75.00% Resodyn IJ7-015 Resin/IJ7-008 2.83 255 ± 20 123 ± 8  35.00% 2.49 4320 ± 290 7600 ± 410 Filler/XJ8-148 (w/30 min 65.00% delayed) IJ7-017 Resin/IJ7-010 35.00% Filler/XJ8-148 65.00% Resodyn IJ7-050 Resin/IJ7-046 2.66 270 ± 18 128 ± 9  35.00% 2.46 3950 ± 350 7170 ± 350 Filler/XJ8-148 (w/30 min 65.00% delayed) IJ7-051 Resin/IJ7-047 35.00% Filler/XJ8-148 75.00% Resodyn IJ7-062A Resin/IJ7-058 2.82 258 ± 14 118 ± 4  35.00% 2.37 3260 ± 180 6170 ± 270 Filler/XJ8-148 (w/30 min 65.00% delayed) IJ7-063 Resin/IJ7-059 35.00% Filler/XJ8-148 65.00% Resodyn IJ7-062B Resin/IJ7-046 2.95 242 ± 27 109 ± 4  35.00% 2.25 2800 ± 410 6100 ± 380 Filler/XJ8-148 (w/30 min 65.00% delayed) IJ7-064 Resin/IJ7-060 35.00% Filler/XJ8-148 65.00%

TABLE 6 Compositions and Properties of Formulated Flowables for Viscosity-increasing Composite Compositions IJ6-005 IJ6-001 IJ6-003 Resin Blend IJ5-208 IJ5-204* IJ5-206* 45.01% 45.01% 45.03% Mol % Thiol: 0.0737 Mol % Mol % Thiol: 0.0737 Thiol: 0.0737 Filler Blend 907445(57) 907445(57) 907445(57) (XJ8-148) 907446(29) 907446(29) 907446(29) 999141(14) 999141(14) 999141(14) 54.99% 54.99% 54.97% Paste No gel soft gel stiff gel Appearance *freshly mixed resin blend for immediate use in paste-making;

Consequently, it was discovered that a remarkably stable pair of methacrylated resin and polythiol (PETMP) could be achieved from EBPADMA during the extensive resin screening study for improved resin stability: no any viscosity increase as measured after 42 days/RT aging (see FIG. 9), in comparison to 10-20 fold of increase in viscosity for the other resin like TPH resin. It was also found UDMA demonstrated better compatibility with PETMP even though there was slight increase (doubled) in viscosity.

Other approach to stabilize polythiol/methacrylated resin system was also examined in TPH resin and SDR resin, respectively, see FIGS. 10 and 11. The inhibitors included PYG, TTBPP, TPP and L-Gallate (Table 2). They were loaded in the resin blend in 1% wt/wt. The preliminary results revealed that the effectiveness of these inhibitors was varied depending upon the methacrylated resin, like TPH resin or SDR resin. PYG appears more effective in inhibiting the viscosity increase in TPH resin system than in SDR resin but discoloration occurred in both resin systems. TTBPP would not work at all in both TPH resin and SDR resin. However, TPP appears working better in SDR resin than in TPH resin; L-Gallate does not work with TPH resin but worked very well in SDR resin system. Therefore both TPP and L-Gallate should be considered as effective additives for SDR resin/PETMP system and none of them worked for TPH resin, unfortunately.

As shown in FIG. 13, EBPADMA/PETMP system is still remaining stable as aged for more than two months at RT. EBPADMA was found stable with THIOCURE PETMP as well as shown in FIG. 14. Thus it was chosen as the resin system for the base paste. To further evaluate the paste stability of such formulated composites, as shown in Table 2, TPH Resin, SDR Resin, Isosorbide Resin and EBPADMA were used as matrix resin in formulations for the catalyst composite paste, in which a hyperbranched polyester acrylate resin (NC2303 from Sartomer) was used as the polyene. These resulting paste/paste flowable composites were evaluated. As expected these formulated resins do demonstrate good stability as aged at room temperature (FIG. 15). Good mechanical properties were also found, see Table 4 and 5, from those pairs of formulated pastes containing SDR Resin (IJ6-057/060), EBPADMA (IJ6-058/060) and Isosorbide Resin (IJ6-059/060), respectively. However, all of these pairs of pastes would not cure well under LED irradiation. It was speculated there was an inefficient thiol/ene Michael addition reaction during the stage one between PETMP and NC2303. Thus there might leave excess PETMP as unreacted thiol prior to light curing, which would act as chain transfer agent that lead to poor crosslinking reaction under LED irradiation. It was expected that under halogen irradiation, however, a light-induced thiol/ene step-addition might occur so as to boost overall crosslinking reaction and no significant impact on mechanical property was found accordingly.

Further as showed in FIG. 16, EBPADMA/PETMP system remains stable as aging for more than three months (98 days) at RT; In addition, Isosorbide resin and EBPADAM are stable with THIOCURE PETMP for more than two months (77 days) at RT. It was also interesting to note that TPH resin is stable with THIOCURE ETTMP though its blend with THIOCURE PETMP is not stable as showed in FIGS. 17 and 18. In Table 2, it is showed the compositions and mechanical properties of additional two series of catalyst pastes that contain both photoinitiators (CQ/LTPO) and thiol/ene catalyst (DBU) in resin blends of various methacrylate resins (TPH Resin, SDR Resin, Isosorbide Resin and EBPADMA) and acrylate resin (TCDCDA or SR295) were formulated and evaluated in an effort to optimize the composition for rapid initial viscosity increasing upon paste/paste mixing. Furthermore, FIGS. 19-24 showed the oscillation profiles of flowable composite (SureFil SDRflow® and universal composite (TPH3) and the experimental paste/paste-based viscosity-increasing flowables that are based on SR295 (IJ6-88/IJ6-92, IJ6-89/IJ6-92, IJ6-90/IJ6-92, and IJ6-91/IJ6-92, respectively). Obviously unlike the conventional composites, both SureFil SDRflow® or TPH3, a distinguished viscosity increasing was demonstrated as evident by the G′/G″ crossover, which is ranged from 50″ to 100″ depending upon the resin composition. In Table 7-8, it is summarized the change of storage modulus (G′), loss modulus (G″) and the complex viscosity (η*). However, for those flowable pairs that are based on TCDCDA (IJ6-74/IJ6-80, IJ6-75/IJ6-80, IJ6-76/IJ6-80, and IJ6-77/IJ6-80), no such pronounced viscosity increasing was found, which might be attributed to the less effective of the diacrylate (TCDCDA) vs the Tetraacrylate (SR295) and the lower concentration of DBU.

TABLE 7 Rheological Property of Viscosity-increasing Flowable Composite Gel time Complex Viscosity Storage Modulus Loss Modulus @ 35° C., η*, Pa · s G′, Pa G″, Pa 175 Pa/1 Hz @30 @30 @30 Paste/Paste second initial min initial min initial min IJ6-088/IJ6-092 52 20 81950 25 500000 120 50000 IJ6-089/IJ6-092 93 15 68045 12 400000 90 20000 IJ6-090/IJ6-092 44 20 73830 35 450000 150 45000 IJ6-091/IJ6-092 73 15 55030 15 300000 100 30000 SureFil SDRflow N/A 37 27 50 25 220 180 TPH3/A2 N/A 280 150 1000 400 1400 800

As discussed previously, it was discovered an effective viscosity—increasing for paste/paste flowable could be achieved upon mixing, as evident by the distinct modulus crossover for EBPADMA/PETMP and a variety of methacrylate resins paired SR295 in presence of DBU. However, no such crossover was found when same mathacryate resin paired with TCDCDA with same amount of DBU. It was speculated that further increase of DBU might boost the thiol/ene reaction for pronounced viscosity-increase. Thus in this month additional DBU, from 0.56% to 1.12% was used in same resin formulation with TCDCDA. Lower mechanical strength was resulted from all composites, which suggests potential negative impact of excess DBU on the free radical polymerization process: showed by both EBPADMA/PETMP and Methacrylate resins (TPH, SDR, EBPADMA and Isosorbide Resin)/TCTCDA if DBU is loaded in 1.12%. Indeed, no modulus crossover occurred for all these formulations.

As showed in Table 5, flowable composites based on EBPADMA/PETMP-EBPADMA/SR295 (IJ6-117/IJ6-118) were formulated by using Resodyn. The mechanical property of such resulting paste/paste composite got improved in comparison to those made via SpeedMix (IJ6-115/IJ6-116, see Table 5). Although the compounding process showed slight impact on the viscosity of the individual flowable, no effect was found on the gel-time during the course of viscosity-increasing process. Accordingly, higher polymerization stress was also resulted due to the reduced porosity in these pastes made via Resodyn. Again, the thiol/ene reaction remains fast, which led to fail in catching up the gel-time at 35° C.

Additional flowable formulations based on EBPADMA/PETMP-TPH Resin/SR295 and EBPADMA/PETMP-EBPADMA/SR295 in presence on reduced DBU (0.86%, wt/wt) and different photoinitiator systems (CQ/EDAB/LTPO vs CQ/LTPO) were formulated as showed Ross mixer and Resodyn (Table 5), respectively. Further improved mechanical properties of such paste/paste composite were evidently resulted for pastes made via Ross Mixer. No significant difference between those pastes containing different photoinitiator systems were found, which confirmed the effectiveness for the CQ/LTPO system in absence of EDAB. It was also found TPH Resin-based system tended to building up the viscosity quickly though there was relative longer gel time. As expected even higher polymerization stress of 3.65 MPa (IJ6-154/IJ6-156 in Table 5) and 3.84 MPa (IJ6-160/IJ6-162 in Table 5) were resulted, which featured in IJ6-154 and IJ6-160 any they derived from same resin, IJ6-149, composing of TPH Resin/SR295 and CQ/EDAB/DBU.

TABLE 8 Compositions and Properties of Flowable Composites@1 Hz Filler Mix Initial Complex Initial Storage Initial Loss Resin Mix IJ7-011 Viscosity@25° C. Modulus@25° C. Modulus@25° C. Composite %, wt/wt %, wt/wt Pa G′, Pa G″, Pa SureFil SDRflow 999308 K900473(58.2)  40 50 220 912401(38.8) 30 20 170 450489(3.0)  31.93   68.07 TPH SPECTRA LV 999445 999117(65.8) 1,900 7,600 9,100 907645(32.9) 600 2,700 2,900 431350(1.3)  24.50   75.50 TPH SPECTRA HV 999445 999117(65.8) 22,600 122,300 71,800 907645(32.9) 54,500 340,900 33,700 431350(1.3)  22.75   77.25 IJ7-012 IJ7-007 907645(40)   70 115 425 907645(60)   45 40 280 Resodyn 35 65 IJ7-013 IJ7-008 907645(40)   85 153 500 907645(60)   50 60 300 Resodyn 35 65 IJ7-014 IJ7-007 907645(40)   85 155 500 907645(60)   50 45 300 Resodyn 35 65 IJ7-015 IJ7-008 907645(40)   75 125 450 907645(60)   50 45 300 Resodyn 35 65 IJ7-016 IJ7-009 907645(40)   55 60 150 907645(60)   20 30 110 Resodyn 35 65 IJ7-017 IJ7-010 907645(40)   25 60 155 907645(60)   20 30 110 Resodyn 35 65 Fillers: 1. BAFG/907445: silanated Ultrafine EG9726, 0.92-0.96 micron 2. BAFG/907446: silanted As-received EG9726, 4-7 microns

TABLE 9 Compositions and Properties of Flowable Composites@1 Hz Initial Complex Initial Storage Initial Loss Resin Mix Filler Mix Viscosity@35° C. Modulus@35° C. Modulus@35° C. Composite %, wt/wt %, wt/wt Pa G′, Pa G″, Pa IJ6-115 IJ6-113 907645(55) 11 12 67 907646(40) 8 8 50 OX-50(5) SpeedMix 40 60 IJ6-116 IJ6-114 907645(55) 21 45 125 907646(40) 15 25 92 OX-50(5) SpeedMix 40 60 IJ6-117 IJ6-113 907645(55) 8 6 50 TPM 1(40) 7 4 40 OX-50(5) SpeedMix 40 60 IJ6-118 IJ6-114 907645(55) 17 30 104 TPM 1(40) 10 12 63 OX-50(5) SpeedMix 40 60 IJ6-139 IJ6-113 907645(55) 10 10 63 907646(40) 9 8 53 OX-50(5) Resodyn 40 60 IJ6-140 IJ6-114 907645(55) 18 32 107 907646(40) 13 18 79 OX-50(5) Resodyn 40 60 IJ6-141 IJ6-113 907645(55) 7 4 41 TPM 1(40) 6 3 36 OX-50(5) Resodyn 40 60 IJ6-142 IJ6-114 907645(55) 12 14 75 TPM 1(40) 9 7 55 OX-50(5) Resodyn 40 60 Fillers: 1. 999141: silanted OX-50, 2. 907445: silanted UltraFine EG9726, 0.92-0.96 micron 3. 907446: silanted As-received EG9726, 4-7 microns 4. TPM1: 130813_1R(YC9-129), 20.3 microns; BET/4.0

TABLE 10 Compositions and Initial Rheological Properties of Viscosity-increasing Flowable Composites Initial Complex Initial Storage Initial Loss Time at Gel Modulus at Gel Viscosity@25° C. Modulus@25° C. Modulus@25° C. Point@25° C. Point@25° C., Composite Pa Pa Pa Second Pa. RossMixer 34 27 214 98 1,508 IJ6-152n156 RossMixer 20 17 122 48 750 IJ6-153n156 RossMixer 28 22 177 84 1,174 IJ6-154n156 RossMixer 17 16 108 103 715 IJ6-155n156 Resodyn 25 22 154 139 1,345 IJ6-158n162 Resodyn 17 16 108 84 755 IJ6-159n162 Resodyn 24 16 150 134 1,266 IJ6-160n162 Resodyn 16 15 101 97 733 IJ6-161n162 Resodyn 25 25 160 150 997 IJ7-012n016 Resodyn 29 28 180 162 1099 IJ7-013n016 Resodyn 27 28 171 160 1034 IJ6-014n017 Resodyn 25 27 157 210 1056 IJ6-015n017 Resodyn 26 25 162 82 1078 IJ7-050n051 Resodyn 57 63 356 N/A N/A IJ7-052n053 Resodyn 30 21 185 77 1225 IJ7-062An063 Resodyn 30 38 240 78 1585 IJ7-062Bn064

TABLE 11 Compositions and 15 min-set Rheological Properties of Viscosity-increasing Flowable Composites Complex Storage Loss Viscosity@25° C. Modulus@25° C. Modulus@25° C. Composite Composite A Composite B Pa Pa Pa RossMixer IJ6-152 IJ6-156 35,300 218,960 35,450 IJ6-152n156 RossMixer IJ6-153 IJ6-156 51,830 321,500 51,800 IJ6-153n156 RossMixer IJ6-154 IJ6-156 52,960 326,100 66,190 IJ6-154n156 RossMixer IJ6-154 IJ6-156 38,450 239,000 35,350 IJ6-155n156 Resodyn IJ6-158 IJ6-162 50,220 312,960 40,490 IJ6-154n156 Resodyn IJ6-159 IJ6-162 53,390 331,540 51,190 IJ6-155n156 Resodyn IJ6-160 IJ6-162 50,540 314,650 43,090 IJ6-160n162 Resodyn IJ6-161 IJ6-162 50,760 316,400 40,060 IJ6-161n162

It was surprisingly found that the individual catalyst pastes made from RossMixer got gelled by after aging at RT for a couple of weeks though the polythiol base paste made from RossMixer remains stable. However, it was also found that same catalyst pastes made from Resodyn also remain stable, which should be attributed to the thermal degradation of the acrylate resin (SR295). Thus such findings should also suggest that Resodyn process is a better option for compounding those heat-sensitive compositions.

Thus it is concluded that

-   -   Thiol-ene chemistry could be viable approach to         viscosity-increasing system by using a superbase, such as DBU,         for rapid network formation at ambient temperature; Extra DBU do         accelerate the rate of thiol-ene reaction for the         viscosity-increasing compositions, but it might be also related         to the reduced mechanical properties. Further investigation is         needed to clarify the negative factor of DBU and porosity for         the high filler loaded flowable compositions.     -   Polyacrylate resins, such as TCDCDA or SR295, could be used in         the catalyst pastes, in combination with conventional         methacrylate resins, such as TPH resin, SDR resin, Isosorbide         resin and UDMA. No significant advantage for those high purity         of polythiols (THIOCURE PETMP or THIOCURE ETTMP 1300) in         stabilizing those urethane-based methacrylated resins (TPH         resin, SDR resin, Isosorbide resin or UDMA).     -   However, is was discovered that only urethane-free methacrylate         resins, such as EBPADMA, would be the chemically compatible with         polythiol (PETMP). It was also found that additional additives,         like TPP and L-Gallate were effective in stabilizing TPH resin         or SDR resin, respectively.     -   Improved mechanical properties were achieved by compounding the         individual flowable composite in Ross Mixer or Resodyn due to         the reduced porosity. But detsablized base phase was found as a         result of mixing by RossMixer under reduced pressure. 

We claim:
 1. A dental composition comprising: (a) a base paste comprising a polythiol and a (meth) acrylate, and (b) a catalyst paste comprising a polyene, a (meth) acrylate resin, a curing system and a catalyst; wherein the catalyst is capable of promoting thiol-ene reaction at room temperature.
 2. The dental composition according to claim 1, wherein the catalyst paste includes ethoxylated bisphenol A dimethacrylate.
 3. The dental composition according to claim 1, wherein the polyene is selected from the group consisting of tricyclo[5.2.1.0^(2,6)]decanedimethanol diacrylate, pentaerythritol tetraacrylate, polyacrylates and polyvinyl ethers.
 4. The dental composition according to claim 1, wherein the polythiols includes pentaerythritol tetra(3-mercaptopropionate) or ethoxylated-trimethylolpropan tri(3-mercaptopropionate.
 5. The dental composition according to claim 1, further comprising a photoinitiator.
 6. The dental composition according to claim 6, wherein the photoinitiator includes camphorquinone, 2,4,6-trimethylbenzoyl diphenylphosphine oxide or mixtures thereof.
 7. The dental composition according to claim 1, further comprising an additive.
 8. The dental composition according to claim 8, wherein the additive includes lauryl gallate or triphenylphosphite.
 9. The dental composition according to claim 1, wherein when the catalyst paste includes ethoxylated bisphenol A dimethacrylate and base paste includes pentaerythritol tetra(3-mercaptopropionate), the composition is capable of being polymerized by irradiation of a light of from 320 nm to 480 nm, even in the absence of any photoinitiator in the dental composition.
 10. The dental composition according to claim 1, further comprising a glass filler in a concentration of from 10 to 70 weight percent based on the total weight of the composition.
 11. The dental composition according to claim 1, further comprising a nanosilica.
 12. The dental composition according to claim 1, wherein the dental composition does not include a photoinitiator. 